1 Journal of Scientific & Industrial Research Vol. 67, September JOHNSON 2008, pp. et al: AGRO WASTES AS LOW COST ADSORBENTS FOR METAL FROM WASTEWATER 647 Agricultural and agro-processing wastes as low cost adsorbents for metal removal from wastewater: A review Thomas Anish Johnson, Niveta Jain*, H C Joshi and Shiv Prasad Division of Environmental Sciences, Indian Agricultural Research Institute, New Delhi Received 29 June 2007; 20 June 2008; accepted 01 July 2008 This study reviews the use of agricultural and agro-processing industry wastes as metal adsorbents from wastewater. Modified materials displayed better adsorption capacity and capability of some was comparable with that of commercial activated carbons and synthetic resins. Agricultural wastes are low-cost adsorbents and can be viable alternatives to activated carbon for treatment of metal-contaminated wastewater. Keywords: Adsorption, Agricultural waste, Low-cost adsorbents, Metals Introduction Heavy metals discharge into aquatic ecosystems is a matter of concern. Eleven metals [lead (Pb), chromium (Cr), mercury (Hg), uranium (U), selenium (Se), zinc (Zn), arsenic (As), cadmium (Cd), cobalt (Co), copper (Cu), nickel (Ni)], out of 20 classified metals as toxic, are emitted into environment in quantities that pose risks to human health 1. Inputs of these trace metals into ecosystem are largely as a result of mining operations, refining ores, sludge disposal, fly ash from incinerators, processing of radioactive materials, metal plating, or manufacture of electrical equipment, paints, alloys, batteries, pesticides and preservatives 2. Presence of heavy metals in environment has become a major threat due to their bio-accumulating tendency and toxicity. Hence, it is necessary to remove these metals from industrial effluents before discharging aqueous waste into environment. Traditional metal removal methods 3 (chemical precipitation, lime coagulation, ion exchange, reverse osmosis and solvent extraction) have certain disadvantages (incomplete metal removal, high reagent and energy requirements, generation of toxic sludge or other waste products). Most of these methods are often ineffective or uneconomical when heavy metal *Author for correspondence Tel: , Fax: concentration is higher ( mg l -1 ) than permissible concentration 4 (< 1 mg l -1 ). Studies 5-13 are available on use of adsorbents for removal of metal ions from effluents. Commercial activated carbon (CAC) is widely used for adsorbing various substances from industrial wastewater However, CAC is expensive material for heavy metal removal 17. Mofa 18 found plant based phytochelatins and proteins bind metals and reduce toxicity. Live biological systems work well for low concentrations but cannot survive high concentrations in highly contaminated areas and industrial effluents 19. Use of non-living bio-materials as metal-binding agents or natural biopolymers are industrially attractive because of their capability in lowering metal ion concentration to parts per billion (ppb) levels due to their high affinity for cationic metals 9,20. Natural materials and certain wastes from agricultural operations have potential to be used as low cost adsorbents 21. Wide variety of agricultural wastes studied as adsorbent for decontaminating industrial/domestic wastewaters from toxic metals, include walnut waste 22, apple waste 23, maize cobs 24, peanut shell 25, 26, cassava waste 27, 28, jackfruit peels 29, fluted pumpkin waste 30, 31, olive pomace 32, wheat bran 33, coconut shell 7, coir pith 34-37, rice husk and bagasse 38. This paper reviews the use of agricultural wastes as metal adsorbents (Tables 1-6)..
2 648 J SCI IND RES VOL 67 SEPTEMBER 2008 Table 1 Cadmium (II) adsorption capacities (q m ) of agricultural waste materials Material q m, mg/g E/K model Bengal gram husk F, L Bengal gram husk L Cassava tuber bark wastes Cassava waste 44 (thioglycolic acid modified) Cocoa shell Coffee residues 124 (pyrolyzed) 39.5 L Coffee wastes Coir pith activated carbon L Corncobs Cornstarch L Jack fruit peel Rs, L F (Sips) Palm sheath 138 (petiolar felt-sheath) 10.8 Peanut hulls Peanut hulls pellets Pinus pinaster bark Rice husk L Rice husk Ps, L Rice husk 93 (NaOH treated) 20.2 Ps, L Rice husk 93 (epichlorohydrin treated) 11.1 Ps, L Rice husk 93 (NaHCO 3 treated) 16.2 Ps, L Sawdust of Pinus silvestris Ps, L Spent grain Ps, L Sterculia lychnophera seeds Sugar beet pulp P, L Sugar cane bagasse pith Ps, L Tea wastes F Tea wastes 113 (binary system) 2.59 F Wheat bran L E/K, Equilibrium/ Kinetic; F, Freundlich; L, Langmuir; Rs, Modified Ritchie second-order; Ps, Pseudo second order Agricultural Wastes as Low Cost Metal Adsorbents Bagasse Bagasse, an agricultural waste from sugar industry, has been found as low cost metal adsorbent. Mohan & Singh 39 studied potentiality of activated carbon (AC) derived from bagasse for removal of Cd (II) and Zn (II) from aqueous solutions in single as well as multi-metal systems. Cd (II) adsorption was slightly more than Zn (II) and increased sorption capacity was reported with increase in temperature. Adsorption on bagasse-based AC occurs through a film diffusion mechanism at all concentrations 39. Using bagasse-based carbon, Ayyappan 40 studied adsorbent of Pb (II) under batch adsorption. Desorption of Pb (II) from sorbed carbon was achieved by eluting with 0.1M HNO 3. Carbon was Table 2 Chromium adsorption capacities (q m ) of agricultural waste materials Material q ma, mg/g E/K model Chitosan on acid treated palm shell charcoal * L Coir pith * Ps, L Rice husk * Rice husk ash 99 (heated at 300 C) 19.09* Rice husk ash 99 (heated at 600 C) 6.49* Rice whole with husk * Cocoa shell ** Almond shell F, L Bagasse F, L Bengal gram husk F, L Coconut husk fibers Coconut shell activated carbon 48 (HNO 3 oxidized) F, L Coconut shell activated carbon 48 (H 2 SO 4 oxidized) 8.94 F, L Coconut shell charcoal 48 (chitosan coated) 3.65 F, L Coconut shell charcoal 48 (HNO 3 oxidized) F, L Coconut shell charcoal 48 (H 2 SO 4 oxidized) 4.05 F, L Eucalyptus bark Fo(L), F Hazelnut shell activated carbon L Olive cake F, L Palm pressed fibers Pine needles F, L Rice husk F Rice husk 98 (ethylene diamine modified) 23.4 Saw dust Sawdust of maple F, L Saw dust F, L Soya cake F, L Sugar beet pulp Sugar cane Bagasse Tamarind hull Pf, F, R-P, F-S Tamarind seed 133 (crushed) 90 Forkf, F a Values indicate maximum amount of Cr (VI) adsorbed (qm) at equilibrium unless otherwise mentioned, *Values for total chromium - Cr (III) + Cr (VI), **Values for Cr (III) E/K, Equilibrium/ Kinetic; F, Freundlich; L, Langmuir; Rs, Modified Ritchie second-order; Pf, Pseudo-first-order; Ps, Pseudo second order; R-P, Redlich-Peterson; F-S, Fritz-Schlunder; Fo(L), First order (Lagergren); Forkf, First order reversible kinetic fit model retrieved by washing with 0.1M CaCl 2 solution and reused. Similar studies were carried with chromium also 38. Bengal Gram Husk Use of bengal gram husk (BGH) (Cicer arientinum L.), a milling agro waste, in single, binary and ternary
3 JOHNSON et al: AGRO WASTES AS LOW COST ADSORBENTS FOR METAL FROM WASTEWATER 649 Table 3 Copper (II) adsorption capacities (q m ) of agricult ural waste materials Material q m, mg/g E/K model Banana peel F Banana pith carbon L Bengal gram husk F, L Cassava tuber bark wastes Cassava waste 44 (thioglycolic acid modified) Cocoa shell Coir activated L Coconut husk Coir pith Cotton seed hull carbon Oil Palm fiber Orange peel F Peanut hull carbon L Peanut hulls Peanut hulls pellets Pecan shells 121 (phosphoric modified) Pecan shell carbon 120 (H 3 PO 4 activated) 6.84 F Pecan shell carbon 120 (CO 2 activated) F Pecan shell carbon 120 (steam-activated) F Sago industry waste Ps Sawdust Soybean hull 131 (citric acid modified) Sugar beet pulp F, L Tea wastes F Tea wastes 113 (binary system) 6.65 F E/K, Equilibrium/ Kinetic; F, Freundlich; L, Langmuir; Ps, Pseudo second order systems of metal solutions was investigated 41,42. Adsorbent removed heavy metal ions (Pb>Cd>Zn>Cu>Ni) efficiently from aqueous solutions and adsorption of metal increased with increasing atomic weight and ionic radii 42. Adsorption of metal ions increased with increase in initial metal concentration. Maximum concentration of heavy metals adsorbed at equilibrium (30 min) was: Pb, 49.97; Cd, 39.99; Zn, 33.81; Cu, 25.73; and Ni, mg g -1 BGH biomass. Maximum adsorption occurred at ph 5. Efficiency of adsorbent to remove Pb (II) from binary and ternary solutions with Cd, Cu, Ni and Zn was of the same level as it was with single solution. Ahalya et al 2 demonstrated removal of 99.9% of chromium in 10 mg l -1 chromium solution using 1 g BGH. Adsorption equilibrium reached within 180 min Table 4 Nickel (II) adsorption capacities (q m ) of agricultural waste materials Material q m, mg/g E/K model Almond husk activated carbon L Bagasse F, L Banana peel F Bengal gram husk F, L Cocoa shell Coir fibers L Coir fibers 50 (H 2 O 2 oxidized) 4.33 L Coir pith Coir pith activated carbon L Coir pith Ps, L Corncobs Fluted pumpkin waste L Fluted pumpkin waste 30 (0.5 N 2- mercaptoethanoic acid modified) 40 L Fluted pumpkin waste 30 (1 N 2- mercaptoethanoic acid modified) L Hazelnut shell activated carbon L Orange peel F Orange peel Pf Peanut hulls L, La Tea wastes L, F Wheat bran Wood ash of rubber tree L, F, Pf E/K, Equilibrium/ Kinetic; F, Freundlich; L, Langmuir; La, Lagergren; Pf, Pseudo first order; Ps, Pseudo second order at optimum ph (2). Adsorption capacity increased with increase in agitation speed. Fourier transform infrared spectroscopy (FTIR) study revealed dominance of hydroxyl and carboxyl groups in adsorption process. Cassava Waste Cassava tuber, a major staple food in Africa and many other parts of world 43, generates enormous waste biomass. Pure activated and differentially thiolated cassava waste biomass 19 (0.5 M and 1 M thiolation level respectively), studied using equilibrium sorption, removed metals from aqueous solutions at following sorption rates: Cd (II), , 0.109; Cu (II), , ; and Zn (II), min -1, min -1. Increased thiolation led to increased incorporation or availability of more binding groups onto cellulosic matrix, which improved adsorptivity of cassava waste biomass. Cassava tuber bark wastes (CTBW) in pure and chemically modified forms had good potential as metal ion adsorbents from aqueous solutions and industrial effluents. From solutions containing 100 mg l -1 of metal, CTBW removed: Cd, 45.61; Cu, 54.21; and Zn, mg g -1. Acid treatment of biomass enhanced sorption capacity 46 (> 50%).
4 650 J SCI IND RES VOL 67 SEPTEMBER 2008 Sorption of Cd (II), Cu (II) and Zn (II) on to pure and thioglycolicolic acid treated CTBW, studied using batch sorption technique 46 at 30 C, was fast and stable. Monolayer sorption capacity for Langmuir isotherm ranged as follows: Cd (II), ; Cu (II), ; and Zn (II), mg g -1. Coconut Wastes Coconut Shell and Fibre Coconut shell based AC 47 removed 66% Cd (II) from water within 80 min at ph 6. Coconut shell charcoal (CSC) oxidized with nitric acid had higher Cr adsorption capacities (10.88 mg g -1 ) than that oxidized with sulfuric acid (4.05 mg g -1 ) or coated with chitosan (3.65 mg g -1 ). Surface modification of CSC with a strong oxidizing agent and treatment of chitosan generated more adsorption sites on its surface for metal adsorption 48. Regeneration of CSC with NaOH and HNO 3 enabled the same column for multiple uses in subsequent cycle with more than 95% regeneration efficiency 49. Shukla et al 50 found that metal uptake of H 2 O 2 modified coir fibres was 4.33, 7.88 and 7.49 mg g -1 for Ni (II), Zn (II) and Fe (II), respectively as against 2.51, 1.83 and 2.84 mg g -1 respectively for unmodified ones due to generation of carboxylic acid groups on fibre. Lowering of ph decrease metal uptake. Unground and unmodified coir 51 in batch sorption removed Zn (91%) and Pb (97%). Coir Pith Adsorption of Cu (II) from aqueous solutions on carbonized coirpith 52 was highest at 25 min [initial Cu (II) concentrations, mg l -1 ]. Removal increased from 50% to 90% with increase of ph from 2.0 to 4.0 and remained constant upto ph 10 for a Cu (II) concentration of 20 mg l -1. Adsorption of metals on coirpith AC from real industrial wastewater was also studied 35,53. Using industrial wastewater containing Cd (II), Ni (II) and Cu (II) ions, maximum metal adsorption 35 occurred at ph At initial ph (5.0) at 30 C for particle size ¼m, adsorption capacities were: Ni (II) 36, 62.5; and Cd (II) 37, 93.4 mg g -1. Adsorption of Ni (II) and Cd (II) increased with ph from 2.0 to 7.0 and remained constant up to At adsorbate concentration of 20 mg l -1, ZnCl 2 activated coir pith carbon 54 is an effective sorbent of Cr (VI), V (V), Ni (II) and Hg (II). Coir pith was also used for adsorption of Co (II), Cr (III) and Ni (II) from single-ion solutions as well as from a mixture 55. Optimum ph for maximum metal-ion adsorption was determined as 4.3 for Co (II), 3.3 for Cr (III) and 5.3 for Ni (II). Table 5 Lead (II) adsorption capacities (q m ) of agricultural waste materials Material q m, mg/g E/K model Barley straw Bengal gram husk L Bengal gram husk F, L Coir F, L, Ps, Fo (L) Coir fibers F, L Hazelnut shell F, L Hop leaf & stem biomass Maize bran L Oil palm shell activated carbon Dlsc Rice husk Rice husk Sago industry waste Ps Sterculia lychnophera seeds E/K, Equilibrium/ Kinetic; F, Freundlich; L, Langmuir; First order (Lagergren); Pf, Pseudo first order; Ps, Pseudo second order; Dlsc, Diffuse layer surface complexation model Table 6 Zinc (II) adsorption capacities (q m ) of agricultural waste materials Material q m, mg/g E/K model Almond husk activated carbon 116 (with H 2 SO 4 ) F, L Almond husk activated carbon with heat F, L Banana peel F Barley straw Bengal gram husk F, L Cassava tuber bark wastes Cassava waste 44 (thioglycolic acid modified) Cocoa shell Coir fibers Coir fibers L Coir fibers 50 (H 2 O 2 oxidized) 7.88 L Orange peel F Peanut hulls 25 9 Peanut hulls pellets Pecan shell carbon 120 (H 3 PO 4 activated) 13.9 F Pecan shell carbon 120 (CO 2 activated) 6.62 F Pecan shell carbon 120 (steam-activated) 7.38 F Sugar beet pulp F E/K, Equilibrium/ Kinetic; F, Freundlich; L, Langmuir
5 JOHNSON et al: AGRO WASTES AS LOW COST ADSORBENTS FOR METAL FROM WASTEWATER 651 Maximum adsorption capacity of coir pith was found to be: Co, 12.82; Cr, 11.56; and Ni, mg g -1. Oil Palm Waste Palm oil industry generates huge amounts of palm shell. Most research on palm shell carbon is focused on carbonization and activation Oil palm shell, because of inherent high densities and carbon content 56,58,59,64, produced high quality AC. Othman et al 65 investigated adsorption of Cd (II) and Pb on modified oil palm shell. Chu & Hashim reported application of palm oil fuel ash for removal of Cr and Zn (II) from aqueous solutions. Biosorbent prepared by coating chitosan onto acid treated oil palm shell charcoal (AOPSC) was studied for Cr removal from industrial wastewater 17. AOPSC (particle size µm) with approx. 21% w/w chitosan loading gave sorption of 154 mg Cr g -1 of chitosan used at 25 C. Palm shell AC 68 showed high adsorption capacity for Pb ions (95.2 mg g -1 ) at ph 5.0. Addition of boric acid to the solution improved total metal uptake, while malonic acid decreased uptake due to formation of Pb-malonate complex. Olive Waste from Oil Production Adsorption efficiency of dried olive husks has been found up to 90% for Zn (II) and Cu (II) ions 69. Increase in initial ph and decrease in particle size enhanced adsorption process. Presence of high concentration of sodium ions strongly suppressed uptake of Zn (II) ions. Pagnanelli et al 70 conducted preliminary studies for removal of different heavy metals (Hg, Pb, Cu, Zn and Cd), effect of pre-treatments by water and n-hexane on metal removal and regeneration possibility. Adsorption followed an affinity series reflecting hydrolytic properties of metallic ions, and particular affinity for Cu (II), which suggests a general ion exchange mechanism combined with a specific complexation reaction for Cu (II) ions. Adsorbent characterization using potentiometric titration, IR analyses and selective extractions titration modeling suggested carboxylic and phenolic groups as main active sites involved in metal removal 32,71. Under equilibrium and dynamic conditions 72, metal sorption capacity of husk was found in the sequence Pb>Cd>Cu>Zn. In dynamic tests, except for Cu (II), a significant reduction in sorption capacity (Pb, 77%; Cd, 93%; Zn, 68%) was recorded. Sorption tests with suspended olive mill residues evidenced 60% Cu (II) removal from solution 73. Acid regenerated residues achieved about 40% Cu (II) removal in same experimental conditions. Regeneration with EDTA at different concentrations damaged active sites of adsorption. Malkoc 74 found maximum Cr (VI) adsorption by olive pomace at ph 2.0; total sorbed Cr (VI) and equilibrium Cr (VI) uptake decreased with increasing flow rate, and increased with increasing inlet Cr (VI) concentration. Olive stone waste 75 used as biosorbent for Pb (II), Ni (II), Cu (II) and Cd (II), gave maximum metal sorption at ph Highest uptake was found for Cd (II) ( molg -1 ) followed by Pb (II) ( molg -1 ), Ni (II) ( molg -1 ) and Cu (II) ( molg -1 ). An increase in ionic strength concentration caused a decrease in metal removal. Orange Wastes Orange peel adsorbed heavy metals from wastewater 76,77. Ajmal et al 78 employed orange peel for Ni (II) removal from simulated wastewater. Maximum metal removal (158 mg g -1 ) occurred at ph 6.0 and 50 C. This result was significantly higher than a similar study by Annadurai et al 79, suggesting that adsorption capacity of an adsorbent depends on initial concentration of adsorbate. Pavan et al 80 using Ponkan mandarin (Citrus reticulata Blanco) peel as biosorbent got maximum adsorption at ph 4.8 from aqueous solutions as follows: Ni (II), 1.92; Co (II), 1.37; and Cu (II) 1.31 mmol g -1. Dhakal et al 81 used orange juice residues to prepare adsorption gel (Ca 2+ form and H + form gels) for metal ions by simple chemical modification. Ca 2+ form gel was effective for complete and selective removal of Pb (II), Cu (II) and Fe (III) compared with other divalent metal ions [selectivity order of gel: Pb (II)>Fe (III)>Cu (II)>Cd (II)>Zn (II)>Mn (II)]. Maximum loading capacities for divalent metal ions [Pb (II), Cd (II) and Zn (II)] were evaluated as 1.1 mol/kg dry gel, while 1.55 mol/kg dry gel for Fe (III). The H + form gel showed a different adsorption profile for Fe (III) compared to Ca 2+ form gel. Both gels were effective at acidic ph. Peanut Waste Peanut shells AC can used to adsorb various metal ions Peanut hulls removed Ni (II) maximum (53.65 mg g -1 ) at ph 4-5 from synthetic solution 85. In column studies, Periasamy & Namasivayam 86 observed maximum Cu (II) removal (65.57 mg g -1 ) at ph 6-10 Cu (II) from synthetic solution using peanut hull. Metal removal by peanut hull in column studies was higher than that in batch studies 25,87. Cu (II) uptake onto peanut hulls and peanut hull pellets was optimum within ph range
6 652 J SCI IND RES VOL 67 SEPTEMBER in batch systems and column studies 26. The capacity of palletized peanut hulls was higher than that of unmodified peanut hulls. Brown et al 25 reported a slight reduction in rate of Cu (II) adsorption on to pellets than on raw peanut hulls but equilibrium capacity was found to be unaffected. Acid treated peanut shells for metal [Cu (II), Ni (II), Zn (II), Cd (II) and Pb (II)] showed higher adsorption (19-34%) from aqueous solution as compared with only 5.7% for non-acid treated samples 90. Chamarthy et al 91 reported that adsorption efficiencies of individual metal ions on modified peanut shells for Cd (II), Cu (II), Ni (II), Pb (II) and Zn (II) ions were at par/ higher than commercial resins Duolite GT-73, Amberlite IRC-718 and carboxymethylcellulose. Wilson et al 88 used peanut shells for adsorption of Cd (II), Cu (II), Pb (II), Ni (II) and Zn (II). Johns et al 89 reported that granular AC produced from peanuts by a combination of CO 2 or steam activation followed by air oxidation, was excellent adsorbent for metal pollutants. Granular AC made from peanut shells adsorbed Cd (II), Cu (II), Ni (II), Pb (II) and Zn (II) ions to a greater extent than comparable CACs. Amounts of Cu (II), Zn (II) and Ni (II) ions adsorbed onto peanut shell 92 increased while that of Cr (VI) ions decreased with increasing equilibrium ph of solution. Maximum uptake of Cr (VI) ions was found at a ph below the point of zero charge of adsorbent (ph[pzc]) and vice versa for Cu (II), Zn (II) and Ni (II). The amount of metal cation adsorbed at given equilibrium concentration increased in the order: Ni (II) < Zn (II) < Cu (II). Peanut shell AC is effective for metal cations at ph e>ph[pzc] and anions at ph d>ph[pzc]. Rice Husk Rice husk has good metal affinity and has potential for use as a low cost sorbent 93. Roy et al 94 demonstrated applicability of ground rice hulls for adsorption of heavy metals [As, Cd, Cr, Pb (>99%) and Sr (94%)]. Maximum Cr (VI) removal (23.4 mg g -1 ) by rice husk AC from aqueous solution is reported 95 at ph 2.0. Chemical pretreatment of rice husk showed varied degree of effects in adsorbing heavy metal from solution 95,96. Daifullah et al 97 used rice husk in removal of metals from a complex matrix containing six heavy metals (Fe, Mn, Zn, Cu, Cd and Pb) and metal removal efficiency of sorbent was approx. 100%. Modified rice husk was investigated for Cr (VI) removal from simulated solution 98. Maximum adsorption capacities of untreated rice with husk (URH), rice husk (RH), rice husk ash heated at 300 C (RHA- 300) and 600 C (RHA-600) were 0.12, 0.50, and 6.49 mgcr g -1 adsorbent, respectively and 0.47, 294, and 4.90 mgbi g -1 adsorbent, respectively, showing RHA- 300 as the most effective adsorbent 99. At optimum conditions (ph 4.0, flow rate 8.0 ml min 1 and particle size d 355 ¼m), 30 g of husks was necessary to attain permissible limits 100 for effluent release for Al, Cd, Cu, Pb and Zn. Batch adsorption of Cd (II) from wastewater with modified rice husk 93 showed that sorption capacity increased from 8.58 mg g -1 (raw rice husk, RRH) to 11.12, and mg g -1 and reduced equilibrium time from 10 h for RRH to 2, 4 and 1 h for epichlorohydrin treated rice husk (ERH), NaOH treated rice husk (NRH) and sodium bicarbonate treated rice husk (NCRH) respectively. Bhattacharya et al 101 observed that adsorption of Zn (II) was maximum with 10 g l -1 rice husk at ph 5-7. Zulkali et al 102 investigated optimum conditions (initial metal concentration, 50 mg l -1 ; temperature, 60 C; biomass loading, 0.2 g; and ph, 5.0) for maximum uptake (98.11%) of Pb (II). Sawdust Several reseachers reviewed sawdust as adsorbent for metals and other pollutants from water. Ajmal et al 106 observed that phosphate treatment of sawdust from mango tree, used for Cr (VI) removal from electroplating wastewater, improved adsorption capacity (100% adsorption at ph<2 and initial concentration of 8-50 mg l -1 ). Almost 87% of sorbed chromium was recovered by treating with 0.01 M NaOH. Adsorptiondesorption cycles 107 showed that Cu (II) binding capacity of sawdust stabilized at 3.1x10-2 meq g -1. Competitive ion exchange exhibited in adsorption from mixture of ions showed order of affinity for sawdust as Ni (II) < Zn (II) < Cd (II) <Cu (II) < Pb (II). Desorption of Pb (II) from sorbed carbon from sawdust 40 was achieved by eluting with 0.1 M HNO 3. Carbon could be retrieved by washing with 0.1 M CaCl 2 solution and reused. Sciban et al 108 examined kinetics of Cu (II), Zn (II) and Cd (II) adsorption on poplar wood sawdust from electroplating wastewater. Adsorption of Cu (II) ions from a mixture was better than that from a single metal solution. Zn (II) showed no change while Cd (II) adsorption was lower in mixture than in single metal solution, due to a difference in binding affinity between ions that reinforces competitive nature of adsorption 107. Sugarbeet Pulp Batch adsorption of sugarbeet pulp 109 (SBP) reached equilibrium by 60 min of contact and achieved 60%
7 JOHNSON et al: AGRO WASTES AS LOW COST ADSORBENTS FOR METAL FROM WASTEWATER 653 removal of Cu (II) and Zn (II); a highest up to 30.9 mg g -1 for Cu (II) at ph 5.5 and 35.6 mg g -1 for Zn (II) at ph 6.0. In another study 110, sugarbeet pulp AC, with initial Cd concentrations of 100, 250 and 500 mg l -1 at 120 min, 20 C, ph 6.3 and adsorbent dose of 2.5 g l -1, removed Cd as 99.0, 78.2 and 57.0% respectively. Reddad et al 111 studied Ni (II) and Cu (II) binding properties of raw and sugar beetpulp modified by saponification, hot 0.05 M HCl and cold 0.05 M NaOH extractions. Baseextracted pulp and saponified pulp exhibited highest Ni (II) and Cu (II) ion removal. Tea Factory Waste Malkoc & Nuhoglu 112 observed mg Ni (II) g -1 adsorption on tea waste at 25 C and initial ph of 4.0. Adsorption reactions were spontaneous ( G <0), slightly endothermic ( H >0) and irreversible ( S >0). Maximum adsorption capacities of Cu (II) and Cd (II) of Turkish tea waste 113 were 8.64±0.51 and 11.29±0.48 mg/g for single and 6.65±0.31 and 2.59±0.28 mg/g for binary systems, respectively. Wastes from Tree Nuts Hasar 114 found maximum Ni (II) adsorption (37.17 mg g -1 ) from simulated solution using almond husk AC at ph 5.0. Ni (II) adsorption capacity of almond husk (37.17 mg g -1 ) was almost four times than that of Cr (VI) adsorption by almond shell 115 (10.67 mg g -1 ) because cell walls of almond husk contain a higher concentration of cellulose, silica and lignin than those of almond shell. Almond husk has more hydroxyl and carboxylic groups than almond shell for metal adsorption, resulting in higher metal removal by almond husk 114. AC from almond husks 116 at optimum conditions (initial metal conc. 20 mg l -1, ph 5.5, temp. 700 C, contact time 60 min and adsorbent conc. 4 g l -1 ) removed 92% of Zn (II) ions Demirbas et al 117 observed that hazelnut shell AC removed from simulated solution maximum Ni (II) (initial metal conc. 15 mg l -1 ) at ph 3.0 with metal adsorption capacity of mg g -1. In another study 118, hazelnut shell was also employed for Cr (VI) adsorption from simulated solution [ph 1, initial Cr (VI) conc mg l -1 ]. Kinetic models for adsorption of Ni (II) ions on to hazelnut shell AC have been compared 119. Pseudo-second order kinetic model correlated better to the data from batch reactions (initial metal ion conc., mg dm -3 ; agitation speed, rpm; and particle size, mm). Treated pecan shells 120 [PSA (phosphoric acidactivated pecan shell carbon), PSC (carbon dioxideactivated pecan shell carbon); PSS (steam-activated pecan shell carbon)] have good removal capacities for Cu (II) and Zn (II) ions removal from real wastewater. At ph 3.6, adsorption capacity of pecan shells 121 for Cu (II) (95 mg g -1 ) was higher than that of SR5 resins (80 mg g -1 ). At ph higher than 8.5, pecan shells had an adsorption capacity of 180 mg g -1, almost two times higher than that at ph 3.6. This measured Cu (II) adsorption capacity was not a reliable result since, at ph higher than 8.5, Cu (II) ions precipitated in the form of hydroxide, thus increasing metal removal from solution. Miscellaneous Materials Jatropha (Jatropha curcas L.) seed coat 122, due to electrostatic attraction of Cu (II) towards lignocellulosic polar groups, removed Cu (II) (82-89%) in 80 min. Jatropha oil cake 123 showed maximum Cr (VI) adsorption at ph 2. Pyrolized coffee residue 124 removed from synthetic solution of metals in the order of Cd (II) > Cu (II) >Zn (II) >Ni (II). Sorption on 2% grape stalks encapsulated in calcium alginate beads was examined in a continuous packed bed column 125. Total uptake decreased with increasing flow rate and increased with increasing inlet Cr (VI) concentration. Charred jackfruit peel made by sulphuric acid treatment was used to study Cd (II) removal from aqueous solution 29. Cocoa shells 126 (15 g l -1 ) adsorbed 161 mmol kg -1 of Pb from aqueous solutions. Horsfall & Spiff 30 assessed differential sorption behaviour of pure and acid treated fluted pumpkin (Telfairia occidenalis Hook. f.) waste biomass on the adsorption of Ni (II) ion from aqueous solution. Hop plant (Humulus lupulus L.) was employed for removal of lead (II) ions from contaminated aqueous solutions 127. Batch adsorption study was carried for Cd (II) removal using shelled moringa (Moringa oleifera Lam.) seed powder 128. Sago processing waste was used to adsorb Pb (II), Cu (II) 129 and Hg (II) 130 ions from aqueous solution. Soybean hull 131 pretreated with NaOH and citric acid, remarkably improved its metal removal capacity. Using tamarind hull 132, removal of chromium enhanced from 33% to 99% with a ph change from 5.0 to 1.0. Crushed tamarind seeds have been used as chromium biosorbent 133. Singh et al 33 reported that wheat bran removed maximum Cd (II) (87.15%) at ph 8.6, initial Cd (II) concentration of 12.5 mg l -1 and temperature 20 C. Singh et al 134 used maize bran for optimum removal of Pb (II) (98.4%) at 20 C, ph 6.5 and initial metal concentration 100 mg l -1.
8 654 J SCI IND RES VOL 67 SEPTEMBER 2008 Comparison of Metal Adsorption Capacities of Adsorbents from Agro-wastes with CAC Adsorption capacities of low coat adsorbents were found to be comparable and in some cases better than that of CAC. Materials like citric acid modified soybean hull 131 [Cr (VI), mg g -1 ], maize bran ( mg Pb(II) g -1 ) 134, orange peel (158 mg Ni(II) g -1 ) 78, chitosan coated on acid treated palm shell charcoal (154 mg Cr(VI) g -1 ) 17, oil palm shell AC (95.2 mg Pb(II) g -1 ) 68, coir pith (91.63 Ni(II) g -1 ) 35 coir pith AC (93.4 mg Cd(II) g -1 ) 37 are found to have superior metal adsorbing capabilities when compared with CAC [Cd(II) 146 mg g -1, Cr(VI) 145 mg g -1, Cu(II) mg g -1, Pb(II) 41 mg g -1, Zn(II) 20 mg g -1 ] 120,147,161,163. Thus, low coat adsorbents from agricultural wastes are good for substituting CAC. Conclusions Agricultural wastes, being porous and lightweight due to fibrous nature, are non-conventional low cost adsorbents for metal adsorption. Carboxylic and hydroxyl functional groups on surface of agricultural wastes have high affinity for heavy metal ions. Physicochemical modifications of wastes can enlarge surface area, type of adsorbing sites, porosity etc, thus improving sorptive capacity, which may compensate for the cost of additional processing. Regeneration of spent adsorbent has become a cost effective and sound environmental option. Desorption and regeneration can be done to recover valuable metal from spent adsorbent. Hydroxyl and carboxylic groups in agricultural wastes make them amenable to easy desorption and regeneration with basic or acid solutions. Acknowledgement T A Johnson thanks CSIR for award of JRF. References 1 Kortenkamp A, Casadevall M, Faux S P, Jenner A, Shayer R O J, Woodbridge N & O Brien P, A role for molecular oxygen in the formation of DNA damage during the reduction of the carcinogen chromium (VI) by glutathione, Arch Biochem Biophys, 329 (1996) Ahalya N, Kanamadi R D & Ramachandra T V, Biosorption of chromium (VI) from aqueous solutions by the husk of Bengal gram (Cicer arientinum), Electron J Biotechnol, 8 (2005); / index.html. 3 Rich G & Cherry K, Hazardous Waste Treatment Technologies (Pudvan Publishing Co, Northbrook) 1987, Holan Z R, & Volesky B, Biosorption of Pb and Ni by biomass of marine algae, Biotechnol Bioeng, 43 (1994) Volesky B, Holan, Z.R.. Biosorption of heavy metals Biotech. Prog, 11 (1995) Ahalya N, Ramachandra T V & Kanamadi R D, Biosorption of Heavy Metals, Res J Chem & Environ, 7 (2003) Pino G H, Mesquita L M S, Torem M L & Pinto G A S, Biosorption of Cd (II) by green coconut shell powder, Minerals Eng, 19 (2006) Namasivayam C, Adsorbents for the treatment of wastewaters, In Encyclopedia of Environmental Pollution and Control, vol I, edited by R K Trivedy (Enviro-media, Karad, India) 1995, Bailey S E, Olin T J, Bricka R M & Adrian D D, A review of potentially low-cost sorbents for heavy metals, Water Res, 33 (1999) Babel S & Kurniawan T A, Low-cost adsorbents for heavy metals uptake from contaminated water: a review, J Hazard Mater, B97 (2003) Kurniawan T A, Chan G Y S, Lo W & Babel S, Comparisons of low-cost adsorbents for treating wastewaters laden with heavy metals, Sci Total Environ, 366 (2006) Mohan D & Pittman C U Jr, Activated carbons and low cost adsorbents for remediation of tri- and hexavalent chromium from water, J Hazard Mater, 137 (2006) Crini G, Recent developments in polysaccharide-based materials used as adsorbents in wastewater treatment, Prog Polym Sci, 30 (2005) Monser L & Adhoum N, Modified activated carbon for the removal of Cu (II), Zn (II), chromium, and cyanide from wastewater, Sep Purif Technol, 26 (2002) Shim J W, Park S J & Ryu S K, Effect of modification with HNO 3 and NaOH by pitch based activated carbon fibers, Carbon, 39 (2001) Ouki S K, Neufeld R D & Perry R, Use of activated carbon for the recovery of chromium from industrial wastewaters, J Chem Technol Biotechnol, 70 (1997) Nomanbhay S M & Palanisamy K, Removal of heavy metal from industrial wastewater using chitosan coated oil palm shell charcoal, Electron J. Biotechnol, 8 (2005); index.html. 18 Mofa A S, Plants proving their worth in toxic metal cleanup, Science, 269 (1995) Abia A A, Horsfall M Jnr & Didi O, Studies on the use of agricultural by-product for the removal of trace metals from aqueous solutions, J Appl Sci Environ Manage, 6 (2002) Gloaguen V & Morvan H, Removal of heavy metal ions from aqueous solution by modified barks, J Environ Sci Health A, 32 (1997) Deans J R & Dixon B G, Uptake of Pb 2+ and Cu 2+ by novel biopolymers, Water Res, 26 (1992) Randall J M, Reuter F C & Waiss A C, Removal of cupric ions from solution by contact with peanut skins, J Appl Polym Sci, 19 (1974) Maranon E & Saatre H, Heavy metal removal in packed beds using apple wastes, Bioresour Technol, 38 (1998) Okiemenn F E, Maya A O & Oriahkhi C O, Sorption of Cd (II), Pb (II) and Zn (II) ions on sulphur containing chemically
9 JOHNSON et al: AGRO WASTES AS LOW COST ADSORBENTS FOR METAL FROM WASTEWATER 655 modified cellulosic materials, Int J Environ Anal Chem, 32 (1998) Brown P, Jefcoat I A, Parrish D, Gill S & Graham E, Evaluation of the adsorptive capacity of peanut hull pellets for heavy metals in solution, Adv Environ Res, 4 (2000) Johnson P D, Watson M A, Brown J & Jefcoat I A, Peanut hull pellets as a single use sorbent for the capture of Cu (II) from wastewater, Waste Manage, 22 (2002) Horsfall M Jr & Abia, A A, Sorption of Cd (II) and Zn (II) ions from aqueous solutions by cassava waste biomass (Manihot esculenta Cranz), Water Res, 37 (2003) Horsfall M Jr, Spiff A I, & Abia, A A, Studies on the influence of mercaptoacetic acid (MAA) modification of cassava (Manihot esculenta Cranz) waste biomass on the adsorption of Cu 2+ and Cd 2+ from Aqueous Solution, Bull Korean Chem Soc, 25 (2004) Inbaraj B S & Sulochana N, Carbonised jackfruit peel as an adsorbent for the removal of Cd (II) from aqueous solution, Biores Technol, 94 (2004) Horsfall M Jr & Spiff A I, Effect of 2-mercaptoethanoic acid treatment of fluted pumpkin waste (Telfairia occidentalis Hook. f.) on the sorption of Ni 2+ ions from aqueous solution, J Sci Ind Res, 64 (2005) Horsfall M Jr & Spiff A I, Sorption of Pb (II), Cd(II) and Zn(II) on sulphur- containing chemically modified wastes of fluted pumpkin (Telfairia occidentalis Hook. f.), Chem Biodiversity, 2 (2005) Pagnanelli F, Mainelli S, De-Angelis S & Toro L, Biosorption of protons and heavy metals onto olive pomace, Modelling of competition effects, Water Res, 39 (2005) Singh K K, Talat M & Hasan S H, Low cost biosorbent wheat bran for the removal of Cd (II) from wastewater: Kinetic and equilibrium studies, Biores Technol, 97 (2006) Namasivayam C & Kadirvelu K, Agricultural solid wastes for the removal of heavy metals, Adsorption of Cu (II) by coir pith carbon, Chemosphere, 34 (1997) Kadirvelu K, Thamaraiselvi K & Namasivayam C, Removal of heavy metals from industrial wastewaters by adsorption onto activated carbon prepared from an agricultural solid waste, Biores Technol, 76 (2001) Kadirvelu K, Thamaraiselvi K & Namasivayam C, Adsorption of nickel (II) from aqueous solution onto activated carbon prepared from coir pith, Sep Purif Technol, 24 (2001) Kadirvelu K & Namasivayam C, Activated carbon from coconut coir pith as metal adsorbent: adsorption of Cd (II) from aqueous solution, Adv Environ Res, 7 (2003) Sarin V & Pant K K, Removal of chromium from industrial waste by using eucalyptus bark, Biores Technol, 97 (2006) Mohan D & Singh K P, Single- and multi-component adsorption of Cd(II) and Zn(II) using activated carbon derived from Bagasse an agricultural waste, Water Res, 36 (2002) Ayyappan R, Carmalin-Sophia A, Swaminathan K. & Sandhya S, Removal of Pb (II) from aqueous solution using carbon derived from agricultural wastes, Process Biochem, 40 (2005) Saeed A, Iqbal M & Akhtar M W, Removal and recovery of lead (II) from single and multimetal (Cd, Cu, Ni, Zn) solutions by crop milling waste (black gram husk), J Hazard Mater, 117 (2005) Saeed A, Akhtar M W & Iqbal M, Affinity relationship of heavy metal biosorption by the husk of Cicer arietinum (chickpea var. black gram) with their atomic weights and structural features, Fresenius Environ Bull, 14 (2005) Osagie A U, Antinutritional Factors in Nutritional Quality of Plants (University of Benin press) 1998, Abia A A, Horsfall M & Didi O, The use of chemically modified and unmodified cassava waste for the removal of Cd, Cu, and Zn ions from aqueous solution, Biores Technol, 90 (2003) Horsfall M Jr, Abia, A A & Spiff A I, Removal of Cu (II) and Zn (II) ions from wastewater by cassava waste biomass (Manihot esculenta Cranz), Afr J Biotechnol, 2 (2003) Horsfall M Jr, Abia, A A & Spiff A I, Kinetic studies on the adsorption of Cd 2+, Cu 2+ and Zn 2+ ions from aqueous solutions by cassava (Manihot esculenta Cranz) tuber bark waste, Biores Technol, 97 (2006) Gaikwad R W, Removal of Cd (II) from aqueous solution by activated charcoal derived from Coconut shell, Electron J Environ Agric Food Chem, 3 (2004) Babel S & Kurniawan T A, Cr (VI) removal from synthetic wastewater using coconut shell charcoal and commercial activated carbon modified with oxidizing agents and/or chitosan, Chemosphere, 54 (2004) Kurniawan T A, A research study on Cr (VI) removal from electroplating wastewater using chemically modified low-cost adsorbents and commercial activated carbon, Master thesis, Sirindhorn International Institute of Technology (SIIT), Thammasat University, Bangkok, Shukla S R, Pai R S & Shendarkar A D, Adsorption of Ni (II), Zn (II) and Fe (II) on modified coir fibers, Sep Purif Technol, 47 (2006) Conrad K & Hansen H C B, Sorption of Zn (II) and lead on coir, Biores Technol, 98 (2007) Namasivayam C & Kadirvelu K, Coir pith an agricultural by product for the treatment of dyeing wastewater, Biores Technol, 48 (1994) Santhy K & Selvapathy P, Removal of heavy metals from wastewater by adsorption on coir pith activated carbon, Sep Sci Technol, 39 (2004) Namasivayam C & Sangeetha D, Recycling of agricultural solid waste, coir pith: Removal of anions, heavy metals, organics and dyes from water by adsorption onto ZnCl 2 activated coir pith carbon, J Hazard Mater, 135 (2006) Parab H, Joshi S, Shenoy N, Lali A, Sarma U S & Sudersanan M, Determination of kinetic and equilibrium parameters of the batch adsorption of Co (II), Cr (III) and Ni (II) onto coir pith, Process Biochem, 41 (2006) Hussein M Z, Tarmizi R S H, Zainal Z, Ibrahim R & Badri R M, Preparation and characterization of active carbons from oil palm shells, Carbon, 34 (1996) Lua A C & Guo J, Preparation and characterization of chars from oil palm waste, Carbon, 36 (1998)
10 656 J SCI IND RES VOL 67 SEPTEMBER Guo J & Lua A C, Preparation and characterization of adsorbents from oil palm fruit solid wastes, J Oil Palm Res, 12 (2000) Guo J & Lua A C, Adsorption of sulphur dioxide onto activated carbons prepared from oil palm shells impregnated with potassium hydroxide, J Chem Technol Biotechnol, 75 (2000) Guo J & Lua A C, Textural and chemical properties of adsorbent prepared from palm shell by phosphoric acid activation, Mater Chem Phys, 80 (2003) Guo G, The effect of local hydrodynamics on mass transfer in disordered porous media, Ph D Dissertation, Louisiana State University, USA, Daud W M A W, Ali W S W & Sulaiman M Z, effect of activation temperature on pore development in activated carbon produced from palm shell, J Chem Technol Biotechnol, 78 (2002) Daud W M A W & Ali W S W, Comparison of pore development of activated carbon produced from palm shell and coconut shell, Biores Technol, 93 (2004) Normah M, Teo K C & Watkinson A P, Preparation and characterization of activated carbon derived from oil palm shells using a fixed bed pyrolyser, in Bioproducts Processing: Technologies for the Tropics, edited by M A Hashim (Institute of Chemical Engineers, Rugby, United Kingdom) 1995, Othman F, Salim M R & Ahmad R, MOPAS for metal removal, in 20 th WEDC Conf (Colombo, Sri Lanka) 1994, Chu K H & Hashim M A, adsorption and desorption characteristics of Zn(II) on ash particles derived from oil palm waste, J Chem Technol Biotechnol, 77 (2002) Chu K H & Hashim M A, Adsorption characteristics of trivalent chromium on palm oil fuel ash, Clean Technol Environ Policy, 4 (2002) Issabayeva G, Aroua M K & Sulaiman N M N, Removal of lead from aqueous solution on palm shell activated carbon, Biores Technol, 97 (2006) Al-Asheh S & Banat F, Adsorption of Zn (II) and Cu (II) Ions by the solid waste of the olive oil industry, Adsorp Sci Technol, 19 (2001) Pagnanelli F, Toro L & Veglio F, Olive mill solid residues as heavy metal sorbent material: a preliminary study, Waste Manage, 22 (2002) Pagnanelli F, Mainelli S, Veglio F & Toro L, Heavy metal removal by olive pomace, biosorbent characterization and equilibrium modeling, Chem Eng Sci, 58 (2003) Volpe A, Lopez A & Pagano M, Olive husk: an alternative sorbent for removing heavy metals from aqueous streams, Appl Biochem Biotechnol, 110 (2003) Veglio F, Beolchini F & Prisciandaro M, Sorption of Cu (II) by olive mill residues, Water Res, 37 (2003) Malkoc E, Nuhoglu Y & Dundar M, Adsorption of chromium (VI) on pomace-an olive oil industry waste: Batch and column studies, J Hazard Mater, 138 (2006) Fiol N, Villaescusa I, Martínez M, Miralles N, Poch J & Serarols J, Sorption of Pb (II), Ni (II), Cu (II) and Cd (II) from aqueous solution by olive stone waste, Sep Purif Technol, 50 (2006) Selvakumari G, Murugesan M, Pattabi S & Sathishkumar M, Treatment of electroplating industry effluent using maize cob carbon, Bull Environ Contam Toxicol, 69 (2002) Azab M S & Peterson P J, The removal of Cd (II) from water by the use of biological sorbants, Water Sci & Technol, 21 (1989) Ajmal M, Rao R A K, Ahmad R & Ahmad J, Adsorption studies on Citrus reticulata (fruit peel of orange) removal and recovery of Ni (II) from electroplating wastewater, J Hazard Mater, 79 (2000) Annadurai A, Juang R S & Lee D J, Adsorption of heavy metals from water using banana and orange peels, Water Sci Technol, 47 (2003) Pavan F A, Lima I S, Lima E C, Airoldi C & Gushikem Y, Use of Ponkan mandarin peels as biosorbent for toxic metals uptake from aqueous solutions, J Hazard Mater, 137 (2006) Dhakal R P, Ghimire K N & Inoue K, Adsorptive separation of heavy metals from an aquatic environment using orange waste, Hydrometallurgy, 79 (2005) Namasivayam C & Periasamy K, Bicarbonate treated peanut hull carbon for mercury (II) removal from aqueous solution, Water Res, 27 (1993) Periasamy K & Namasivayam C, Process development for removal and recovery of Cd (II) from wastewater by a low cost adsorbent: adsorption rate and equilibrium studies, Ind Eng Chem Res, 33 (1994) Periasamy K & Namasivayam C, Adsorption of Pb (II) by peanut hull carbon from aqueous solution, Sep Sci Technol, 30 (1995) Periasamy K & Namasivayam C, Removal of nickel (II) from aqueous solution and nickel planting industry wastewater using agriculture waste: peanut hulls, Waste Manage, 15 (1995) Periasamy K & Namasivayam C, Removal of Cu (II) by adsorption onto peanut hull carbon from wastewater and Cu (II) plating industry wastewater, Chemosphere, 32 (1996) Rao M, Parawate A V & Bhole A G, Removal of Cr 6+ and Ni 2+ from aqueous solution using Bagasse and fly ash, Waste Manage, 22 (2002) Wilson K, Yang H, Seo C W & Marshall W E, Select metal adsorption by activated carbon made from peanut shells, Biores Technol, 97 (2006) Johns M M, Marshall W E & Toles C A, Agricultural by products as granular activated carbons for adsorbing dissolved metals and organics, J Chem Technol, 71 (1998) Wafwoyo W, Chung W S & Marshall W E, Utilization of peanut shells as adsorbents for selected metals, J Chem Technol Biotechnol, 74 (1999) Chamarthy S, Chung W S & Marshall W E, Adsorption of selected toxic metals by modified peanut shells, J Chem Technol Biotechnol, 76 (2001) Romero L C, Bonomo A & Gonzo E E, Peanut shell activated carbon: Adsorption capacities for Copper (II), zinc (II), nickel (II) and chromium (VI) ions from aqueous solutions, Adsorp Sci Technol, 22 (2004) Kumar U & Bandyopadhyay M, Sorption of Cd (II) from aqueous solution using pretreated rice husk, Biores Technol, 97 (2006)
11 JOHNSON et al: AGRO WASTES AS LOW COST ADSORBENTS FOR METAL FROM WASTEWATER Roy D, Greenlaw P N & Shane B S, Adsorption of heavy metals by green algae and ground rice hulls, J Environ Sci Health A, 28 (1993) Bishnoi N R, Bajaj M, Sharma N & Gupta A, Adsorption of Cr (VI) on activated rice husk carbon and activated alumina, Biores Technol, 91 (2004) Ajmal M, Rao R A K, Anwar S, Ahmad J & Ahmad R. Adsorption studies on rice husk: removal and recovery of Cd (II) from wastewater, Biores Technol, 86 (2003) Daifullah A A M, Girgis B S & Gad H M H, Utilization of agroresidues (rice husk) in small waste water treatment plans, Materials Lett, 57 (2003) Tang P L, Lee C K, Low K S & Zainal Z, Sorption of Cr (VI) and Cu (II) in aqueous solution by ethylenediamine modified rice hull, Environ Technol, 24 (2003) Bakircioglu Y, Bakircioglu D & Akman S, Solid phase extraction of bismuth and chromium by rice husk, J Trace & Microprobe Technique, 21 (2003) Ricardo C, Tarley T & Arruda M A Z, Biosorption of heavy metals using rice milling by-products, Characterization and application for removal of o:metals from aqueous effluents, Chemosphere, 54 (2004) Bhattacharya A K, Mandal S N & Das S K. Adsorption of Zn(II) from aqueous solution by using different adsorbents, Chem Eng J, 123 (2006) Zulkali M M D, Ahmed A L & Norulakmal N H. Oryza sativa L. husk as heavy metal adsorbent: Optimization with lead as model solution, Biores Technol, 97 (2006) Shukla A, Zhang Y H, Dubey P, Margrave J L & Shukla S S, The role of sawdust in the removal of unwanted materials from water, J Hazard Mater, 95 (2003) Vaishya R C & Prasad S C, Adsorption of Cu (II) on sawdust, Indian J Environ Prot, 11 (1991) Shukla S R & Sakhardande V D, Novel method of using reactive dyestuff for effluent treatment, Am Dyest Rep, 41 (1991) Ajmal M, Rao R A K & Siddiqui B A, Studies on removal and recovery of Cr (VI) from electroplating wastes, Water Res, 30 (1996) Marin J & Ayele J, Removal of some heavy metal cations from aqueous solutions by spruce sawdust II: Adsorption-desorption through column experiments, Environ Technol, 24 (2003) Sciban M, Radetic B, Kevresan Z & Klasnja M, Adsorption of heavy metals from electroplating wastewater by wood sawdust, Biores Technol, 98 (2007) Pehlivan E, Cetin S & Yanik B H, Equilibrium studies for the sorption of Zn (II) and Cu (II) from aqueous solutions using sugar beet pulp and fly ash, J Hazard Mater, 135 (2006) Ozer A, Tanyildizi M S & Tumen F, Study of Cd (II) adsorption from aqueous solution on activated carbon from sugar beet pulp, Environ Technol, 19 (1998) Reddad Z, Gerente C, Andres Y, Ralet M C, Thibault J F, Cloirec P L, Ni (II) and Cu (II) binding properties of native and modified sugar beet pulp, Carbohyd Polym, 49 (2002) Malkoc E & Nuhoglu Y, Investigations of nickel (II) removal from aqueous solutions using tea factory waste, J Hazard Mater, 127 (2005) Cay S, Uyanik A & Ozai K A, Single and binary component adsorption of Cu (II) and Cd (II) from aqueous solutions using tea-industry waste, Sep Purif Technol, 38, (2004) Hasar H, Adsorption of nickel (II) from aqueous solution onto activated carbon prepared from almond husk, J Hazard Mater, B97 (2003) Dakiky M, Khamis M, Manassra A & Mer eb M, Selective adsorption of chromium (VI) in industrial wastewater using lowcost abundantly available adsorbents, Adv Environ Res, 6 (2002) Hasar H, Cuci Y, Obek E & Fatih-Dilekoglu M, Removal of Zn (II) by activated carbon prepared from almond husks under different conditions, Adsorp Sci Technol, 21 (2003) Demirbas E, Kobya M, Oncel S & Sencan S, Removal of Ni (II) from aqueous solution by adsorption onto hazelnut shell activated carbon: equilibrium studies, Biores Technol, 84 (2002) Kobya M, Removal of Cr (VI) from aqueous solutions by adsorption onto hazelnut shell activated carbon: kinetic and equilibrium studies, Biores Technol, 91 (2004) Kobya M, Demirbas E, Oncel M S & Encan S S, Adsorption kinetic models applied to nickel ions on hazelnut shell activated carbons. Adsorp Sci Technol, 20 (2002) Bansode R R, Losso J N, Marshall W E, Rao R M & Portier R J, Adsorption of metal ions by pecan shell-based granular activated carbons, Biores Technol, 89 (2003) Shawabkeh R A, Rockstraw D A & Bhada R K, Cu (II) and strontium adsorption by a novel carbon material manufactured from pecan shells, Carbon, 40 (2002) Jain N, Joshi H C, Dutta S C, Kumar S & Pathak H, Biosorption of copper from wastewater using jatropha seed coat, J Sci Ind Res, 67 (2008) Garg U K, Kaur M P, Garg V K & Sud D, Removal of hexavalent chromium from aqueous solution by agricultural waste biomass, J Hazard Mater, 140 (2007) Boonamuayvitaya V, Chaiya C, Tanthapanicchakoon W & Jarudilokul S, Removal of heavy metals by adsorbent prepared from pyrolyzed coffee residues and clay, Sep Purif Technol, 35 (2004) Fiol N, Escudero C, Poch J & Villaescusa I, Preliminary studies on Cr (VI) removal from aqueous solution using grape stalk wastes encapsulated in calcium alginate beads in a packed bed up-flow column, Reactive & Funct Polym, 66 (2006) Meunier N, Jerome L, Jean-Francois B & Tyagi R D, Lead removal from acidic solutions by sorption on cocoa shells: effect of some parameters, J Environ Eng, 129 (2003) Gardea-Torresdey J, Hejazi M, Tiemann K, Parsons J G, Duarte- Gardea M & Henning J, Use of hop (Humulus lupulus) agricultural by-products for the reduction of aqueous lead (II) environmental health hazards, J Hazard Mater, 91 (2002) Sharma P, Kumari P, Srivastava M M & Srivastava S, Removal of Cd (II) from aqueous system by shelled Moringa oleifera Lam. seed powder, Biores Technol, 97 (2006) Quek S Y, Wase D A J & Forster C F, The use of sago waste for the sorption of lead and Cu (II), Water SA, 24 (1998) Kadirvelu K, Kavipriya M, Karthika C, Vennilamani N & Pattabhi, S, Mercury (II) adsorption by activated carbon made from sago waste, Carbon, 42 (2004)